High strain-rate response of commercially pure High strain-rate response of commercially pure...
Embed Size (px)
Transcript of High strain-rate response of commercially pure High strain-rate response of commercially pure...
High strain-rate response of commercially pure vanadium
Sia Nemat-Nasser *, Weiguo Guo 1
Center of Excellence for Advanced Materials, Department of Mechanical and Aerospace Engineering, University of California,
9500 Gilman Drive, San Diego, La Jolla, CA 92093-0416, USA
Received 1 July 1999; received in revised form 18 October 1999
To understand the plastic ¯ow behavior of commercially pure vanadium under high strain rates, uniaxial com-
pression tests of cylindrical samples are performed using UCSD's enhanced Hopkinson technique. True strains ex-
ceeding 50% are achieved in these tests, over a range of temperature from 77 to 800 K at the strain rates of 2500 and
8000 sÿ1. The microstructure of the deformed and undeformed samples is observed by an optical microscope. The initial microstructure (the initial dislocation density, the grain size and its distribution) is found to have a strong eect on the
yield stress and the initial stages of the ¯ow stress. This eect becomes more signi®cant with decreasing temperature.
Deformation twins are observed. Their density is seen to increase with decreasing temperature. Adiabatic shearbands
occur in vanadium at low temperatures. Finally, an experimentally based micromechanical model is developed for the
dynamic response of this material. The model predictions are compared with the results of other high strain-rate tests
which have not been used in the evaluation of the model parameters, and good agreement between the theoretical
predictions and experimental results is obtained. In addition, the results of a series of low strain-rate tests are presented
and brie¯y discussed. Ó 2000 Elsevier Science Ltd. All rights reserved.
Keywords: Vanadium; Dislocations; Microstructures; Plastic ¯ow; Model
Vanadium, V, is a body-centered-cubic (bcc) crystal, belonging to Group V-A of the Periodic Table. Since its discovery by Manuel Del Rio in 1801 (Kinzel, 1950; Elvers and Hawkins, 1996), it has found broad usage in many ®elds. For exam- ple, it is an important element in steel and Ti al-
loys, and it has applications in the nuclear industry, in medicine, and in superconductor re- search. Like other refractory metals, the mechan- ical properties of vanadium are strongly dependent on its purity and hence on its production method. Its ¯ow stress is a function of temperature, strain rate, and its microstructure, e.g., the dislocation density and distribution. For these reasons, eorts have been made to understand the in¯uence of strain rate, temperature, and the microstructure on the mechanical properties of this material. Com- pared to other refractory metals, some of the re- markable properties of vanadium are: 1. it has more plasticity and its brittle±ductile
transition temperature is rather low;
Mechanics of Materials 32 (2000) 243±260 www.elsevier.com/locate/mechmat
* Corresponding author. Tel.: +1-858-534-5930; fax: +1-858-
E-mail address: email@example.com (S. Nemat-Nasser). 1 Current address: Department of Aircraft Engineering,
Northwestern Polytechnical University, Xi'an 710072, People's
Republic of China.
0167-6636/00/$ - see front matter Ó 2000 Elsevier Science Ltd. All rights reserved. PII: S 0 1 6 7 - 6 6 3 6 ( 9 9 ) 0 0 0 5 6 - 3
2. its stacking-fault formation energy seems to be the lowest among the pure refractory metals with a bcc lattice (Zubets et al., 1978);
3. its slip geometry and dislocation structure ex- hibit distinguishing features, as compared with those of the other bcc refractory metals, be- cause the dislocations in vanadium are more prone to dissociation (Noskova and Dolgopo- lov, 1978). In general, at low strain rates (usually
approximately 120 lm. Compression tests are carried out at strain rates of 2500 and 8000 sÿ1
over a range of temperatures from 77 to 800 K. Room-temperature experiments at high strain rates of 13 500, 20 000, and 30 500 sÿ1 are also performed to check the model predictions. All these dynamic tests are performed using a split Hopkinson pressure bar with a momentum trap (Nemat-Nasser et al., 1991). This novel Hopkin- son bar is also enhanced by a furnace which heats the sample while only minimally aecting the in- cident and the transmission bars (Nemat-Nasser and Isaacs, 1997).
To reduce the end friction on the samples dur- ing a dynamic loading, the sample ends are ®rst polished using waterproof silicon carbide paper, 800±4000 grit, and then they are greased for low- and room-temperature tests. A molybdenum powder lubricant is used for the high-temperature tests. It is known that the oxidation of vanadium becomes serious at temperatures exceeding 250°C (Elvers and Hawkins, 1996). Therefore, an argon atmosphere is used in the heating furnace in order to prevent oxidization.
3. Experimental results and discussion: microstruc-
ture and plastic ¯ow
3.1. Initial microstructure
It is well known that the plastic response of most materials depends on the strain rate and temperature, as well as on the microstructural features such as the grain size, second-phase par- ticles, and the dislocation density and its distri- bution.
3.2. Grain-size distribution
To examine the eect of grain size on the ¯ow stress, samples of vanadium are sectioned, pol-
ished, and then etched in a 12.5 ml HNO3, 2.5 ml HF, 25 ml H2O solution for 3 min. The grain-size distribution is then examined by optical micros- copy. A nonuniform distribution is observed for both as-received and annealed samples. The aver- age grain size in the central one-third portion of the sample is about 10 lm for the as-received and 76 lm for the annealed cases. For the remaining portion of the sample, the corresponding sizes are 17 and 165 lm, respectively. For the purpose of comparison, the average grain sizes of 14 lm for the as-received and 120 lm for the annealed samples, are used. Fig. 1 shows the microstructure of an annealed sample, taken at a two-third di- ameter, within the sample.
3.3. The eect of grain size on plastic deformation
Fig. 2 compares the ¯ow stress of the as-re- ceived and annealed samples, over the indicated temperatures, at a strain rate of 2500 sÿ1. As is seen, only the high-temperature response seems to be aected by the average grain size for strains greater than 20%; see also Fig. 3. The initial dis- location density in the as-received material may be as high as 1012 cmÿ2, while for the annealed sam- ples, it may be as low as 106 cmÿ2 (Edington and Smallman, 1964). Hence, the initial low-tempera- ture ¯ow stress of the as-received material is con- siderably higher than that of the annealed one, because of greater dislocation-impurities and dis- location±dislocation interactions. At room- and high-temperatures, this dierence seems to disap- pear. The eect of the average strain size is seen to become evident for a 700 K initial temperature, as shown in Figs. 2 and 3; this dierence is believed to be due to the eect of the grain size on the long- range resistance to the motion of dislocations.
Fig. 4 displays the ¯ow stress of annealed va- nadium over the temperature range of 77±800 K, at a strain rate of 2500 sÿ1. It is seen that a further increase in temperature above 700 K does not
The major impurities of the polycrystal vanadium
Element N O C H Al Cr Fe Si Mo Ta
ppm 70 200 30 3 140 100 120 250 390 100
S. Nemat-Nasser, W. Guo / Mechanics of Materials 32 (2000) 243±260 245
aect the ¯ow stress at this strain rate, indicating that the response is essentially temperature-inde- pendent for temperatures greater than 700 K.
3.4. Adiabatic shearbands and deformation twins
Adiabatic shearbands are observed in most bcc metals which are deformed at low initial temper- atures and high strain rates, to large strain rates. While vanadium shows greater plasticity than other bcc refractory metals, it does shearband
when deformed to large plastic strains, as shown in Fig. 5(a) and (b), for the as-received and annealed samples, respectively.
Fig. 6 shows the microstructure of the sample shown in Fig. 5(b). The arrow indicates the loading direction; the loading direction is the same in all ®gures. Twinning is observed at low temperatures and high strain rates, as is evident in Fig. 6. The density of twins decreases sharply as the test tem- perature is increased; see Fig. 7(a) and compare with Fig. 6. The higher temperature produces
Fig. 2. Comparison of ¯ow stress between as-received and annealed vanadium.
Fig. 1. Microstructure of an annealed vanadium sample.
246 S. Nemat-Nasser, W. Guo / Mechanics of Materials 32 (2000) 243±260
serrated twins, and this is also evident in Fig. 7(b) which corresponds to the microstructure that re- sults when a sample is ®rst deformed to about c 0:18 at a 77 K initial temperature, and then is heated to a room temperature of 296 K before being loaded at the same 2500 sÿ1 strain rate, by an additional 20% strain. The deformation mecha- nism in vanadium is believed to change from that controlled by the Peierls resistance to the disloca- tion motion at temperatures below about 200 K, to that controlled by the predominant interaction between the dislocations and the interstitial impu- rities (Conrad and Hayes, 1963; Wang and Bain- bridge, 1972), above 200 K. The observed serration
at the edges of the twins at 296 K, may possibly be a result of the intersection of the dislocation-induced slip and the deformation twins. T